انواع روش های بتن ریزی در زیر آب
1.استفاده از بتن پیش آکنده
2. کار با کیسه
3.Non Dispersible Concrete (N.D.C(
4.بتن ریزی با پمپ
5.بتن ریزی با قیف و لوله (تِرِمی)
6.بتن ریزی با جام
Third Straw project on Lake
Mead—one of the largest
U.S. municipal water
Barge-mounted Putzmeister concrete
placing system places 12,000 cu yds
(9,175m³) of concrete underwater to
secure a water intake structure for the
Third Straw project, which will draw
water from the Lake Mead reservoir.
An aerial view of the equipment barge, which staged two complete
concrete placing system setups—one operational, one backup.
Continuous tremie pour lasts 12 days,
with concrete outputs peaking over
100 cu yds an hour (76m³/hr).
Step 1: Ready-mix trucks are loaded on a transport barge, eight at a time,
to deliver concrete for a tremie pour almost three miles from shore.
Step 2: Concrete is discharged from ready-mix trucks onto Maxon conveyors
located on the equipment barge.
Step 3: The concrete is conveyed into a Maxcrete remix surge hopper, which
provided a high capacity to ensure a continuous concrete flow to the BSA 14000
HP-D trailer-mounted pump when transitioning to the next barge of ready-mix
Step 4: A 38-meter Putzmeister placing
boom places the concrete into a
tremie pipe that sends the concrete
390 ft (119m) underwater.
For Structural concrete following
must be considered
Coarse Aggregate: Gravel of 3/4” (20mm) max. size. Use 50-55 % of the
total aggregate by weight.
• Sand, 45-50% of the total aggregate by weight.
• Cement: Type II ASTM (moderate heat of hydration), 600 lbs/yd3
• Pozzolans: ASTM 616 Type N or F, 100 lbs/ yd3
• Water/Cement Ratio: 0.42 (0.45 Maximum).
• ƒWater-Reducing Admixture (preferably it is also plasticizer): Do not use
• ƒAir-Entrainment Admixtures: To give 6% total air.
• ƒRetarding Admixture: To increase setting time to 4-24 hours, as
• ƒSlump: 6 1/2" ± 1"
• ƒThis mix will develop compressive strength in the range of 5,600 – 7,000
psi at 28 days.